NMR, STRUCTURE AND SPECTROSCOPIC INVESTIGATIONS ON …
Research and Reviews in Materials Science and Chemistry Vol. 4, Issue 1, 2014, Pages 17-34 ISSN 2319-6920 Published Online on July 19, 2014 2014 Jyoti Academic Press http://jyotiacademicpress.net Keywords and phrases: cadmium, structure, X-ray, NMR, IR. Communicated by Darina Simedru. Received March 4, 2014; Revised April 30, 2014 NMR, STRUCTURE AND SPECTROSCOPIC INVESTIGATIONS ON A CESIUM-AMMONIUM CADMIUM TRICHLORIDE A. BEN CHRIFA, A. BEN SALAH and M. LOUKIL Laboratoire des Sciences des Matériaux et d’Environnement Faculte des Sciences de Sfax-3018 Tunisie e-mail: [email protected]Abstract The structure of cesium-ammonium cadmium trichloride ( ) , CdCl NH Cs 3 01 . 0 4 0.99 has been determined by X-ray single crystal analysis at room temperature. This material crystallizes in Ia-3 space group with , 8 = Z and unit cell dimension () . 4 4487 . 10 a Å = Several cycles of least squares refinement reduced the disagreement R(F) factor for 342 reflections to a final value of 0.01 and 2 R W for 0.05. The compound structure consists of ( ) + + 4 NH or Cs ions and 6 CdCl octahedra ensuring the stability of the structure by ionic and hydrogen bonding contacts N–H…Cl. The + 4 NH substitution gives more orientation disorder in the structure at room temperatures. IR and Raman spectroscopy studied at room temperature were performed to confirm results of the X-ray diffraction.
NMR, STRUCTURE AND SPECTROSCOPIC INVESTIGATIONS ON …
Text of NMR, STRUCTURE AND SPECTROSCOPIC INVESTIGATIONS ON …
Research and Reviews in Materials Science and Chemistry Vol. 4, Issue 1, 2014, Pages 17-34 ISSN 2319-6920 Published Online on July 19, 2014 2014 Jyoti Academic Press http://jyotiacademicpress.net
Keywords and phrases: cadmium, structure, X-ray, NMR, IR. Communicated by Darina Simedru. Received March 4, 2014; Revised April 30, 2014
NMR, STRUCTURE AND SPECTROSCOPIC INVESTIGATIONS ON A CESIUM-AMMONIUM
A. BEN CHRIFA, A. BEN SALAH and M. LOUKIL
Laboratoire des Sciences des Matériaux et d’Environnement Faculte des Sciences de Sfax-3018 Tunisie e-mail: [email protected]
The structure of cesium-ammonium cadmium trichloride ( ) ,CdClNHCs 301.040.99
has been determined by X-ray single crystal analysis at room temperature. This material crystallizes in Ia-3 space group with ,8=Z and unit cell dimension
( ) .44487.10a Å= Several cycles of least squares refinement reduced the
disagreement R(F) factor for 342 reflections to a final value of 0.01 and 2RW for
0.05. The compound structure consists of ( )++4NHorCs ions and 6CdCl
octahedra ensuring the stability of the structure by ionic and hydrogen bonding
contacts N–H…Cl. The +4NH substitution gives more orientation disorder in
the structure at room temperatures. IR and Raman spectroscopy studied at room temperature were performed to confirm results of the X-ray diffraction.
A. BEN CHRIFA et al. 18
Compounds based on cadmium have attracted much attention because of their applications in optics and acoustics. These materials are also of special interest because they undergo structural transitions [1-5]. Crystals of 3ABCl family (A being alkali and B = Cd, Mn), undergo
phase transitions to structures that are slightly distorted from ideal Perovskite-type structures [6, 7]. The phase transition temperatures and the structures of the 3ABCl (A = Cs and B = Cd, Mn) crystals are
different from one another, but their phase transition mechanisms are distinguished as the quadruple and magnetic origin. The differences between the chemical properties of Cd and Mn are attributed to the nature of the phase transitions of these crystals. Therefore, the relaxation mechanisms of these different types of 3ABCl crystals
(quadruple and magnetic) are completely different NMR behaviour .
Mixed metal halides of the 3ABX type [A = alkali metal, B = divalent
metal ,Cd,Pb 22 …++ and X a halogen] belong to the Perovskite like
structure, slightly distorted by cation displacements or by tilts of octahedra-BX6 as compared with the ideal cubic structure. The nature
of the distortions is connected with the instability of lattice with respect to one or several vibration modes .
In this paper, we report the structure of ( ) 301.040.99 CdClNHCs at
room temperature in order to examine the effect of the cationic substitution on symmetry related to the ammonium dynamics.
NMR, STRUCTURE AND SPECTROSCOPIC … 19
( ) 301.040.99 CdClNHCs was synthesized by dissolving a mixture of
Cl,NH,CsCl 4 and 2CdCl in hot water, the chemical reaction is
( ) ( ) .CdClNHCsCdClClNHCsCl1 301.0499.0OH
242 →++− xx
Colourless thin rectangular parallelepiped crystals were grown after vapourizing in air for 18 days approximately.
2.2. X-ray structure determination
The crystal structure of ( ) 301.040.99 CdClNHCs was studied using an
APEX II diffractometer with graphite-crystal monochromatic αMoK
radiation ( ).71073.0 Å A total of 342 reflections were collected, among
which only 114 reflections, namely those for which ( ),Fo4Fo σ> were
used to determine and refine the structure. Corrections were made for Lorentz–polarization and absorption effects.
Data collection procedure and structure refinement at room temperature, are given in Table 1.
A. BEN CHRIFA et al. 20
Table 1. Crystal structure data and experimental conditions of structure determination for ( ) 301.040.99 CdClNHCs
The cadmium atoms positions were determined by using a three dimensional Patterson synthesis. Chlorine, nitrogen, and cesium atoms were located by a three-dimensional Fourier function. The H atoms were located geometrically, and attributed isotropic thermal factors equal to those of the atoms on which they are linked. Structure solution and refinement were carried out by using (SHELX) programs [9, 10]. The non-hydrogen atoms were refined anisotropically. The atomic coordinates at room temperature are given in Table 2, the anisotropic displacement parameters in Table 3, the bond lengths and angles in Table 4.
Table 2. Fractional atomic and equivalent thermal parameters
The infrared absorption spectrum was carried out on a Perkin-Elmer
1750 spectrophotometer in the 1cm400-4000 − range on a pellet on
powdered sample dispersed in KBr.
The Raman spectrum of polycrystalline samples sealed in glass tube was recorded on a Horiba Jobin yvon Raman spectrometer T64000 equipped with CCD detector. The spectrum was recorded in the region
1cm10-400 − with a resolution of .cm2 1−
NMRMASCd113 spectra were measured on powdered crystals and
glasses at 63, 637MHz with a Varian UNITY INOVA 400 MAS FT-NMR spectrometer. A single pulse sequence was used; for the crystals a pulse length of ,s2µ the accumulation of 5343 and a pulse delay of 3s. A
cylindrical zirconia rotor in which a sample was put, was rotated at a speed of about 8000Hz. A 1M of ( )24ClOCd aqueous solution was used as
NMR, STRUCTURE AND SPECTROSCOPIC … 25
3. Results and Discussion
3.1. Structure of ( ) 30.0140.99 CdClNHCs description
The crystal structure of ( ) 301.040.99 CdClNHCs is presented in Figure 1.
Figure 1. Projection of the ( ) 301.040.99 CdClNHCs structure.
At room temperature, ( ) 301.040.99 CdClNHCs single crystals have an
cubic structure with eight molecules per unit cell, and belong to the Ia-3 space group. The lattice parameters is ( )Å44487.10a = at 293K. In this cubic phase, each Cd atom is surrounded by six Cl atoms, which form a nearly regular octahedron.
Cadmium atoms are located in the 8(a) sites ( )0,0,0 of the Ia-3 space group, surrounded by an octahedron chlorine atom in the 24(d) positions ( ).,0,0 ¼ The Cs or N atoms occupy also the 8(b) sites ( ).,, ¼¼¼
The +Cs or +4NH tetrahedra, reside in between the octahedra with
Cs/N–H...Cl distances about 3.697(2) Å and Cl–Cs/N–Cl angles varying
from 60° to 180°. The presence of +4NH cations induces the coexistence of
A. BEN CHRIFA et al. 26
H bonding contacts N–H...Cl, which providing a linkage between +4NH
cationic entities and [ ] −46CdCl anionic complexes. Nitrogen or cesium
atoms are nine fold coordinated by Cl atom neighbors (Figure 3).
The nitrogen N occupies the (8b) ( )¼¼¼ ,, Wyckoff position. Therefore to determine the hydrogen positions, there are three probable cases:
● Four special positions (8b or 8a).
● Two special positions (16a).
● One position of multiplicity of 32, is impossible because there is no Wyckoff position with this multiplicity in the Ia-3 space group.
We deduced that it is impossible to apply one of these cases, while taking into account a Å9.0 distance for the N–H bond.
For this reason, it was thought that in this structure the ammonium groups probably have an orientation disorder.
Therefore, two hydrogen atoms were placed in both (48e) general and (16c) special positions selected from the three-dimensional Fourier function, leading to a two-fold disorder model of the ammonium groups.
3.2. Influence of ammonium-substituting on the 3CsCdCl structure
To understand the +4NH substituted effect on halogenocadmate, the
structures of ( ) ,CdClNHCs,CsCdCl 301.040.993 and 34CdClNH materials
Comparison with 3CsCdCl  compound, we can deduce that the title compound crystallizes in the same structure but with a relative increase of the maximal cation-chlorine distances and a decrease of the minimal cation-chlorine distances. This variation is accompanied by a relative contraction of Cd–Cl bonds. The Cd–Cl distance values in ( )Å64.2CsCdCl3  are relatively higher than those in
( ) ( ( ) )Å1612,2CdClNHCs 301.040.99 (Figure 2).
NMR, STRUCTURE AND SPECTROSCOPIC … 27
Figure 2. Cadmium environment.
Figure 3. ++4NHCs environment.
A. BEN CHRIFA et al. 28
However, in the 34CdClNH material , these distances are
slightly shorter than those observed in 3CsCdCl and ( ) 01.040.99 NHCs
( ) ( ) .Å2660.22513.2:CdCl3 − This fact suggests that the 6CdCl
octahedron adopts a rather geometry with shorter Cd–Cl distances in the pure ammonium compound.
Details of lattice parameters and the cell volume of ,CsCdCl3
34CdClNH and ( ) 301.0499.0 CdClNHCs materials are given in Table 5.
The net behaviour is a decrease of the unit cell volume as well as the “‘b” and “c” parameters with partial substituting cesium by ammonium.
Table 5. Lattice parameters, unit cell volume, and interatomic distances for ( ) ,CdClNHCs,CsCdCl 301.040.993 and 34CdClNH samples
To have more information on the crystal structure, we have undertaken a vibrational study by using infrared spectroscopy and Raman scattering. The tentative assignments of the vibrations are based on a comparison of the infrared and Raman spectra of
( ) 301.040.99 CdClNHCs with other compounds based on cadmium .
The Raman and infrared peaks frequencies are quoted in Table 6.
Table 6. Wavenumbers ( )1cm− of the bands observed in the IR and
Raman spectra at 298K of ( ) 301.040.99 CdClNHCs and their tentative
assignments ( ν : stretching; :δ deformation)
Wavenumbers ( )1cm− Raman IR
500 — ( )OH2δ
2934 — ( )+δ 4s NH
1640 — ( )+δ 4s NH
1374 — ( )+δ 4as NH
50 Lattice mode translation —
76 +Cs translation —
95 −Cl translation —
110 2CdCl libration —
147 +4NH translation —
208 +4NH libration
232 ( )ClCd−ν
The IR spectra of ( ) 301.040.99 CdClNHCs (Figure 4) were recorded for
the wave number region between 4000 and .cm400 1− The IR spectra
show, at high wave numbers, a band at 1cm3500 − may be assigned to the
deformation OH2 vibration, and a band observed at 1cm2934 − relative
NMR, STRUCTURE AND SPECTROSCOPIC … 31
to the ( )+δ 4NH stretching modes. The symmetric and asymmetric bending
vibration of ( )+4NH appears in two bands at 1640 and .cm1374 1−
Figure 4. Infrared absorption spectrum of ( ) .CdClNHCs 301.040.99
The Raman spectrum of ( ) 301.040.99 CdClNHCs was recorded in the
external region of the sub-lattice vibrations, 1cm50-400 − (Figure 5).
Compared with mercury compounds , the observed Raman lines at 1cm50 − is associated to the lattice mode translation. The bands at 147
and 1cm208 − correspond to the +4NH libration. The band at 1cm110 −
corresponds to the 2CdCl libration of the layers and the chains. We have
assigned the band at 1cm95 − and the shoulder at 1cm76 − to the
translation mode of −Cl anion and to the translation mode of +Cs cation, respectively.
A. BEN CHRIFA et al. 32
From these vibrational studies, we can confirm the presence of the ammonium groups in the structure.
Figure 5. Low-frequency Raman spectra of ( ) .CdClNHCs 301.040.99
3.4. NMR spectroscopy
( ) 301.040.99 CdClNHCs with a cubic structure is expected to have a
seven-line NMR spectrum due to the quadruple interactions of
( ).27ICd113 = Instead of seven resonance lines, the Cd113 nuclei in
( ) 301.040.99 CdClNHCs produce only one resonance line in the
temperature range 160-400K, as shown in Figure 6. This result indicates that we have only one local structure around the Cd atoms. The same behaviour was detected in cadmium thiocyanate compounds . According to this result provided by the NMR measurements at room temperature, we can confirm the octahedral coordination for cadmium atoms, which confirms the results of the single crystal measurements.
NMR, STRUCTURE AND SPECTROSCOPIC … 33
Figure 6. NMR spectrum for Cd113 in ( ) 301.040.99 CdClNHCs at room
In conclusion, we have successfully prepared a novel substituted halogenocadmate ( ) 301.040.99 CdClNHCs via slow evaporation method.
The crystal structure of the title compound is characterized by 6CdCl
octahedra. The cesium or ammonium cations are inserted between these octahedra ensuring the stability of the structure by ionic and hydrogen bonding contacts N–H...Cl.
The ammonium substitution in 3CsCdCl material gives more disorder
of the ammonium groups in the structure and leads to a decrease of the unit cell volume as well as the ‘‘b” and ‘‘c” parameters. However, we noted an increase of the ‘‘a” parameter. This finding appears to reflect the
difference of between the ionic radii of +Cs and +4NH cations.
In addition, analysis by IR spectroscopy and Raman scattering confirms the presence of ammonium group and 6CdCl octahedra in our
MAS-NMR spectrum of Cd113 confirms the octahedral coordination of cadmium in the structure.
A. BEN CHRIFA et al. 34
 M. Mohammadi and D. Fray, Acta Mater. 57 (2009), 1049.
 W. Ch. Zheng and S. Y. Wu, Physica B 301 (2001), 186.
 J. Dhahri, A. Dhahri, M. Oumezzine, E. Dhahri, M. Said and H. Vincent, J. Alloys Compd. 467 (2009), 44.
 M. B. Bellakki and V. Manivannan, J. Mater. Sci. 45 (2010), 1137.
 M. Yang, Z. Wen-Chen and H. Lv, Spectrochim. Acta A 72 (2009), 515.
 S. Sakida and Y. Kawamoto, J. Phys. Chem. Solids 63 (2002), 151.
 A. R. Lim and S. Y. Jeong, J. Solid State Chem. 178 (2005), 3095.
 F. Hamzaoui, I. Noiret, G. Odou, F. Danede and F. Baert, J. Solid State Chem. 124 (1996), 39.
 G. M. Sheldrick, SHELXS97, Program for the Refinement of Crystal Structures, University of Gottingen, Germany, 1986.
 G. M. Sheldrick, SHELXL97, Program for the Refinement of Crystal Structures, University of Gottingen, Germany, 1997.
 M. M. Rolies and C. J. De Ranter, Acta Cryst. B 34 (1978), 3057.
 W. A. Hart, O. F. Beumel and T. P. Whaley, Pergamon Texts in Inorg. Chem. 13 (1973), 14.
 M. Loukil, A. Kabadou, Ph. Salles and A. Ben Salah, Chem. Phy. 300 (2004), 247.
 K. Eichele and R. E. Wasylishen, Inorg. Chem. 33(13) (1994), 2766.